#------------------------------------------------------------------------------
#$Date: 2016-02-16 21:30:59 +0100 (mar 16 de feb de 2016) $
#$Revision: 176467 $
#$URL: svn://www.crystallography.net/cod/cif/4/33/83/4338361.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4338361
loop_
_publ_author_name
'Černý, Radovan'
'Schouwink, Pascal'
'Sadikin, Yolanda'
'Stare, Katarina'
'Smrčok, L'ubomír'
'Richter, Bo'
'Jensen, Torben R.'
_publ_section_title
;
 Trimetallic borohydride Li3MZn5(BH4)15 (M = Mg, Mn) containing two weakly
 interconnected frameworks.
;
_journal_issue                   17
_journal_name_full               'Inorganic chemistry'
_journal_page_first              9941
_journal_page_last               9947
_journal_paper_doi               10.1021/ic401139k
_journal_volume                  52
_journal_year                    2013
_chemical_formula_structural     'Li3 Mn Zn5 (BH4)15'
_chemical_formula_sum            'B15 H60 Li3 Mn Zn5'
_chemical_formula_weight         625.28
_space_group_IT_number           193
_symmetry_space_group_name_Hall  '-P 6c 2'
_symmetry_space_group_name_H-M   'P 63/m c m'
_cell_angle_alpha                90
_cell_angle_beta                 90
_cell_angle_gamma                120
_cell_formula_units_Z            2
_cell_length_a                   15.3906(27)
_cell_length_b                   15.3906(27)
_cell_length_c                   8.5898(18)
_cell_measurement_temperature    295
_cell_volume                     1762.1(6)
_diffrn_ambient_temperature      295
_diffrn_radiation_wavelength     0.75274
_pd_proc_2theta_range_inc        0.027
_pd_proc_2theta_range_max        31.00
_pd_proc_2theta_range_min        2.1
_pd_proc_wavelength              0.75274
_cod_data_source_file            ic401139k_si_008.cif
_cod_data_source_block           b_Mn_13_2_5
_cod_original_cell_volume        1762.09(72)
_cod_original_sg_symbol_H-M      P_63/m_c_m
_cod_original_formula_sum        'B15 H60 Li3 Mn1 Zn5'
_cod_database_code               4338361
loop_
_symmetry_equiv_pos_as_xyz
'-x, -x+y, -z+1/2'
'-x, -x+y, z'
'-x, -y, -z'
'-x, -y, z+1/2'
'-x+y, -x, -z+1/2'
'-x+y, -x, z'
'-x+y, y, -z'
'-x+y, y, z+1/2'
'-y, -x, -z'
'-y, -x, z+1/2'
'-y, x-y, -z+1/2'
'-y, x-y, z'
'y, -x+y, -z'
'y, -x+y, z+1/2'
'y, x, -z+1/2'
'y, x, z'
'x-y, -y, -z+1/2'
'x-y, -y, z'
'x-y, x, -z'
'x-y, x, z+1/2'
'x, y, -z+1/2'
'x, y, z'
'x, x-y, -z'
'x, x-y, z+1/2'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_symmetry_multiplicity
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_occupancy
_atom_site_B_iso_or_equiv
Zn1 Zn 0 0.3333333 0.6666667 0.25 1 3.93(54)
Zn2 Zn 0 0.28609(43) 0 0.25 1 3.93(54)
Li1 Li 0 0.60885(65) 0 0.25 0.66(1) 0.20(98)
Mn1 Mn 0 0.60885(65) 0 0.25 0.34(1) 0.20(98)
Li2 Li 0 0 0 0 1.000(41) 0.20(98)
B1 B 0 0.1312562 0. 0.25 1 4.0(11)
H11 H 0 0.08901241 0. 0.3579802 1 4.0(11)
H12 H 0 0.1390531 -0.06938794 0.25 1 4.0(11)
B2 B 0 0.3320008 0. 0.001795784 1 4.0(11)
H21 H 0 0.295792 0. -0.1130071 1 4.0(11)
H22 H 0 0.4044797 0. -0.02110249 1 4.0(11)
H23 H 0 0.2791717 -0.06938794 0.07064635 1 4.0(11)
B3 B 0 0.5252469 0.3437408 0.25 1 4.0(11)
H31 H 0 0.4432175 0.2834932 0.25 1 4.0(11)
H32 H 0 0.5316519 0.420331 0.25 1 4.0(11)
H33 H 0 0.5630595 0.3355695 0.1423324 1 4.0(11)
loop_
_audit_conform_dict_name
_audit_conform_dict_location
cif_core.dic ftp://ftp.iucr.org/pub/cif_core.dic
cif_pd.dic ftp://ftp.iucr.org/pub/cif_pd.dic
